Article On Modeling of Synthesis Process of Boron Carbide Based Nanocomposites

Levan Chkhartishvili 1,2,*, Levan Antashvili 1 , Lasha Dalakishvili 1, Roin Chedia 3, Otar Tsagareishvili 1 and Archil Mikeladze 1

1 Ferdinand Tavadze Metallurgy and Materials Science Institute, 10 E. Mindeli Str., Tbilisi 0186, Georgia; [email protected] (L.A.); [email protected] (L.D.); [email protected] (O.T.); [email protected] (A.M.) 2 Department of Engineering Physics, Georgian Technical University, 77 M. Kostava Ave., Tbilisi 0160, Georgia 3 Peter Melikishvili Institute of Physical and Organic Chemistry, 31 A. Politkovskaya Str., Tbilisi 0186, Georgia; [email protected] * Correspondence: [email protected]

Abstract: Nanocomposites based on boron carbide B4C are hard materials with wide ﬁeld of applica- tions in modern technologies. A system of ﬁrst-order ordinary differential equations that simulates

the process of chemical synthesis of nanopowders of B4C–TiB2 compositions containing titanium diboride (TiB2) as an additional phase is suggested and resolved numerically for a typical ratio of reaction constants. Reagents and products concentrations are found as time-functions. In this way, the optimal route of production technology of boron carbide-based nanomaterials can be identiﬁed.

Keywords: modeling; chemical synthesis; liquid charge; nanocomposite; boron compounds

Citation: Chkhartishvili, L.; 1. Introduction Antashvili, L.; Dalakishvili, L.; Chedia, R.; Tsagareishvili, O.; Because of complex properties useful for diverse industrial applications, hard nanocom- Mikeladze, A. On Modeling of posites based on boron carbide (with the approximate chemical formula B4C) serve for an Synthesis Process of Boron Carbide important class of advanced materials. In previous works [1–6], we developed an effective Based Nanocomposites. Condens. method of their chemical synthesizing in nanopowdered form from corresponding liquid Matter 2021, 6, 3. https://doi.org/ charges. As is known (e.g., see [7]), optimization of the parameters of chemical technologies 10.3390/condmat6010003 is possible through their mathematical modeling. Here, we develop a set of ordinary differ- ential equations describing evolution of concentrations of reactants (reagents, intermediate Received: 6 January 2021 substances, and products) of chemical reactions, in which the boron carbide/titanium Accepted: 15 January 2021 diboride B4C–TiB2 nanocomposites are formed. Published: 18 January 2021 In the original technology developed, for boron (B), sources include amorphous boron (a-B), boron oxide (B2O3), or boric acid (H3BO3). A carbon source is some liquid organic Publisher’s Note: MDPI stays neutral compound CxHyOz containing carbon (C), hydrogen (H), and oxygen (O). As for the with regard to jurisdictional claims in titanium (Ti) source, usually a titanium dioxide (TiO2) powder is used for this purpose. published maps and institutional afﬁl- The reagents are obtained in the process of a multi-stage heat treatment of the aqueous iations. suspension of these precursors. The B-containing reagent is always a powder of amorphous boron. Thus, the boron source practically does not change when a-B serves as the precursor material. Organic solvent pyrolysis reduces the most part of carbon into carbon black with turbostratic Copyright: © 2021 by the authors. graphite structure. Besides, carbon is emitted with carbon dioxide (CO2). At temperatures Licensee MDPI, Basel, Switzerland. ◦ higher than ~700 C, C reacts with CO2 forming carbon monoxide (CO): CO2 + C → 2 This article is an open access article CO. Note that the production of a carbide-based composite requires free carbon in excess. distributed under the terms and Under corresponding conditions, C-containing reagents are not CO2 and CO, but C and conditions of the Creative Commons CO. As for carbon, during the heat pretreatment, TiO2 is retained in powdered form almost Attribution (CC BY) license (https:// without changes. creativecommons.org/licenses/by/ 4.0/).

Condens. Matter 2021, 6, 3. https://doi.org/10.3390/condmat6010003 https://www.mdpi.com/journal/condensedmatter Condens. Matter 2021, 6, 3 2 of 13

2. Formally Simple Chemical Reactions Representing Technology According to the standard mathematical modeling method [8] of the technological process, the corresponding physical-chemical transformation has to be imagined as a set of (formally) simple, irreversible, homogeneous, and isothermal chemical reactions conducted in a closed volume. Transformation of reagents B, C, CO, and TiO2 into products B4C and TiB2 seems to occur through the following reactions:

C + TiO2 → TiO + CO↑, (1)

3 CO + TiO → TiC + 2 CO2↑, (2)

2 B + TiC → TiB2 + C, (3)

4 B + C → B4C. (4)

Hence, in addition to boron carbide (B4C) and titanium diboride (TiB2) the product is carbon dioxide (CO2) as well. Free carbon (C) being a reagent in Reactions (1) and (4) is an intermediate substance in Reaction (3). Similarly, carbon monoxide (CO) is a reagent in Reaction (2) and an intermediate substance in Reaction (1). Finally, titanium oxide (TiO)—according to Reactions (1) and (2)—andtitanium carbide (TiC)—according to Reactions (2) and (3)—serve only as intermediate substances. By deﬁnition, the order of a chemical reaction is the total number of particles— “molecules”—participating in an elementary collision act. Therefore, for Reactions (1)–(4), the orders are 2, 4, 3, and 5, respectively. As practice shows, the order of a simple chemical reaction cannot exceed 3 and, therefore, Reactions (2) and (4) seem to be complex. However, the establishment of real, i.e., effective, orders for these reactions requires more detailed consideration of their chemical mechanisms. First, note that the icosahedral cluster B12 is the main structural motif for any con- densed phase of elemental boron (as well as boron-rich compounds), including amorphous boron [9]. It remains stable only in the material’s bulk and, upon (in our case, high- temperature) ablation from the powder particle surface, takes a quasiplanar form with broken bonds and, accordingly, greatly increased chemical activity [10]. For this reason, it is natural to think that, not four individual B atoms, but a B12 quasiplanar cluster en- ter into the reaction. Clusters formation is also characteristic of carbon ablation process. One of the highest mass spectrometric peaks corresponds to C3 clusters [11]. Therefore, the mechanism of Reaction (4) can be represented as the interaction of only two particles: clusters B12 and C3. Similarly, the mechanism of Reaction (3), in which elemental boron also acts as a reagent, seems to be the interaction of B12 cluster with the (TiC)6 fragment of the titanium carbide structure. At high temperatures, in a medium containing both carbon and oxygen, various oxycarbon structures are formed. Among the small oxycarbonic clusters [12], only (CO)3 is metastable and, for this reason, hyperactive chemically. Therefore, the mechanism of Reaction (2) can be imaged as the interaction of a metastable cluster (CO)3 with a fragment of the titanium oxide structure in the form of a diatomic TiO molecule. In its original form, the order of Reaction (1) is already 2. However, it is most likely carried out not by the interaction between C atom and TiO2 molecule [13], but some small carbon cluster, for example the same C3 and the corresponding fragment (TiO2)3 of the titanium dioxide structure. Thus, the production of B4C–TiB2 nanocomposite powder is (formally) represented by the following combination of simple chemical reactions:

C3 + (TiO2)3 → 3 TiO + (CO)3↑, (5)

(CO)3 + TiO → TiC + 2 CO2↑, (6)

B12 + (TiC)6 → 6 TiB2 + 2 C3, (7) Condens. Matter 2021, 6, 3 3 of 13

B12 + C3 → 3 B4C. (8) Note that all of them are of secondorder, since reagents are represented by pairs of clusters. Because all reactants (reagents, intermediates, and products) are in dispersive (nanopowdered or even free cluster) or gaseous forms, their mixing is assumed to be good enough to consider distribution of reactants concentrations in the reaction space, i.e., chamber volume, as almost homogeneous. Now, we have to discuss another key assumption of the model used: chemical close- ness of the reaction chamber or lack of exchange of matter with environment. Most reactants are in the solid phase and, consequently, remain in the chamber during whole technology process. There are only two reactants, CO and CO2, in the gas phase. In Reaction (2), gaseous CO produced from the precursor mixture serves for a reagent together with inter- mediate CO produced in Reaction (1). Thus, at the properly chosen charge composition, no presence of free (not reacted) CO is expected in the system. CO2, the ﬁnal gaseous product, is carried away from the chamber by an inert gas (e.g., argon) ﬂow. As mentioned above, in principle, carbon dioxide can react with carbon. However, at the properly chosen charge composition, no presence of free (not reacted) C is expected. It means that CO2 left in the system would behave as an inert gas and then dispute the exchange of CO2 gas with environment, the reaction chamber effectively remaining closed.

3. Reactions Rates

From the acting masses law, the rates V1, V2, V3, and V4 of second-order chemical Reactions (5)–(8) are square functions of corresponding reagents or intermediates concen- trations (number of formula unit “molecules” per unit volume) [B], [C], [CO], [TiO2], [TiO], and [TiC]: V1 = k1[C][TiO2], (9)

V2 = k2[CO][TiO], (10)

V3 = k3[B][TiC] (11)

V4 = k4[B][C]. (12)

By deﬁnition, the reaction constants k1, k2, k3, and k4 are positive and not dependent on the reagent concentrations. However, their temperature-dependence (Arrhenius law) is quite signiﬁcant, and, when the thermal treatment is not isothermal, reaction constants are also complex time-functions. In the technology under consideration, at the heatingstage, reagents are formed from precursor charge, while the basic chemical Reactions (5)–(8) proceed too slowly. As for the coolingstage, it starts after all the reagents and products are completely consumed and formed, respectively. Therefore, the assumption that the technology is almost isothermal and the corresponding reaction rates are time-constants is acceptable. Such assumption signiﬁcantly simpliﬁes the system of chemical kinetics equations and, consequently, its solution. The rate of change of a reagent concentration is opposite in sign to the reaction rate, i.e., negative. On the contrary, the rate of change of a product concentration should be positive. In both cases, the reaction rate magnitude is multiplied by the stoichiometric coefﬁcients of corresponding reagents. Thus, the partial rates of changing of reactants concentrations with time t are: Condens. Matter 2021, 6, 3 4 of 13

d[C](1) dt = −V1 = −k1[C][TiO2], d[TiO2](1) dt = −V1 = −k1[C][TiO2], d[TiO](1) dt = +V1 = +k1[C][TiO2], d[CO](1) dt = +V1 = +k1[C][TiO2], d[CO](2) dt = −3V2 = −3k2[CO][TiO], d[TiO](2) dt = −V2 = −k2[CO][TiO], d[TiC](2) dt = +V2 = +k2[CO][TiO], d[CO2](2) dt = +2V2 = +2k2[CO][TiO], d[B](3) dt = −2V3 = −2k3[B][TiC], d[TiC](3) dt = −V3 = −k3[B][TiC], d[TiB2](3) dt = +V3 = +k3[B][TiC], d[C](3) dt = +V3 = +k3[B][TiC], d[B](4) dt = −4V4 = −4k4[B][C], d[C](4) dt = −V4 = −k4[B][C], d[B4C](4) dt = +V4 = +k4[B][C].

Here [B4C], [TiB2], and [CO2] are the product concentrations. Summarizing these partial rates, we obtain the total rates of changing in concentrations of all the reactants:

d[B] d[B](3) d[B](4) dt = dt + dt = −2k3[B][TiC] − 4k4[B][C], d[C] d[C](1) d[C](3) d[C](4) dt = dt + dt + dt = −k1[C][TiO2] + k3[B][TiC] − k4[B][C], d[ ] d[TiO2] TiO2 (1) dt = dt = −k1[C][TiO2], d[CO] d[CO](1) d[CO](2) dt = dt + dt = +k1[C][TiO2] − 3k2[CO][TiO], d[TiO] d[TiO](1) d[TiO](2) dt = dt + dt = k1[C][TiO2] − k2[CO][TiO], d[TiC] d[TiC](2) d[TiC](3) dt = dt + dt = k2[CO][TiO] − k3[B][TiC], d[ ] d[B4C] B4C (4) dt = dt = +k4[B][C], d[ ] d[TiB2] TiB2 (3) dt = dt = +k3[B][TiC], d[ ] d[CO2] CO2 (2) dt = dt = +2k2[CO][TiO]. The numbers of “molecules” of intermediate substances reacted and produced per unit time, respectively, are equal each to other, so that the total rates of change in TiO and TiC concentrations are zero: d[TiO] d[TiO] = = 0. dt dt Consequently, the following conditions should be fulﬁlled:

k1[C][TiO2] = k2[CO][TiO] = k3[B][TiC].

4. System of Chemical Kinetics Equations Based on the above consideration, we obtain the system of chemical kinetic equations:

d[B] = −2k [C][TiO ] − 4k [B][C], (13) dt 1 2 4 d[C] = −k [B][C], (14) dt 4 d[TiO ] 2 = −k [C][TiO ], (15) dt 1 2 Condens. Matter 2021, 6, 3 5 of 13

d[CO] = −2k [CO][TiO ], (16) dt 1 2 d[B C] 4 = +k [B][C], (17) dt 4 d[TiB ] 2 = +k [C][TiO ], (18) dt 1 2 d[CO ] 2 = +2k [C][TiO ]. (19) dt 1 2

If we denote [B] ≡ N1(t), [C] ≡ N2(t), [TiO2] ≡ N3(t), [CO] ≡ N4(t), [B4C] ≡ N5(t), [TiB2] ≡ N6(t), and [CO2] ≡ N7(t), this system takes the new form:

dN (t) 1 = −4k N (t)N (t) − 2k N (t)N (t), (20) dt 4 1 2 1 2 3 dN (t) 2 = −k N (t)N (t), (21) dt 4 1 2 dN (t) 3 = −k N (t)N (t), (22) dt 1 2 3 dN (t) 4 = −2k N (t)N (t), (23) dt 1 3 4 dN (t) 5 = +k N (t)N (t), (24) dt 4 1 2 dN (t) 6 = +k N (t)N (t), (25) dt 1 2 3 dN (t) 7 = +2k N (t)N (t). (26) dt 1 2 3 From these equations, it is clear that total rates of change in concentrations of reagents (N1(t), N2(t), N3(t), and N4(t)) and products (N5(t), N6(t), and N7(t)) are deﬁnitely negative and positive, respectively. Thus, they are monotonously decreasing or increasing functions of time. Accordingly, at the relevant choice of charge composition at the ﬁnal (t = ∞) and initial (t = 0) time moments, respectively, these concentrations are expected to equal zero:

N1(∞) = N2(∞) = N3(∞) = N4(∞) = N5(0) = N6(0) = N7(0) = 0. (27)

5. Initial Conditions To solve the system of ﬁrst-order ordinary differential equations describing the reagent and product concentration evolution with time, it is necessary to provide their concen- trations at the initial (t = 0) and ﬁnal (t = ∞) time moments, respectively: N1(0), N2(0), N3(0), N4(0), N5(∞), N6(∞), and N7(∞). Note that some of these values can be related to each other. Let us introduce the stoichiometric coefﬁcients 1 − x and x for the product (B4C)1−x(TiB2)x components, where x < 1. Thus,

N (∞) 1 5 = − 1. N6(∞) x

Since boron carbide- (not titanium diboride-)based composites are considered, the inequality 1 − x > x or x < 1/2 must hold. Analogously, if 1 − y and y, where y < 1, are the stoichiometric coefﬁcients of the reagent components: C1−y(CO)y, i.e., COy, the following relation must hold: N (0) 1 2 = − 1. N4(0) y Condens. Matter 2021, 6, 3 6 of 13

If N denotes the ﬁnal concentration of the product’s basic component—boron carbide (B4C)—then: N5(∞) = N.

That of the product’s other component—titanium diboride (TiB2)—is: xN N (∞) = . 6 1 − x To ﬁnd the rest of initial conditions, we need mass balance relations for all reagent and product constituents’ chemical elements—B, C, Ti, and O. As [B]0 initial and [B]∞ ﬁnal concentrations of boron are equal:

2(2 − x)N 2(2 − x)N N (0) = [B] = [B] = 4N (∞) + 2N (∞) = ,N (0) = . 1 0 ∞ 5 5 1 − x 1 1 − x

As [C]0 initial and [C]∞ ﬁnal concentrations of carbon are equal:

N2(0) + N4(0) = [C]0 = [C]∞ = N + N7(∞),N2(0) + N4(0) − N7(∞) = N.

As [Ti]0 initial and [Ti]∞ ﬁnal concentrations of titanium are equal: xN N (0) = [Ti] = [Ti] = N (∞),N (0) = N (∞) = . 3 0 ∞ 6 3 6 1 − x

As [O]0 initial and [O]∞ ﬁnal concentrations of oxygen are equal: 2xN 2xN + N (0) = 2N (0) + N (0) = [O] = [O] = 2N (∞),2N (∞) − N (0) = . 1 − x 4 3 4 0 ∞ 7 7 4 1 − x From theabove-obtained system of three equations for three unknown quantities N2(0), N4(0), and N7(∞), we ﬁnd their values:

2yN 2(1 − y)N (1 + x − (1 − x)y)N N (0) = ,N (0) = ,N (∞) = . 2 (1 − x)(1 + y) 4 (1 − x)(1 + y) 7 (1 − x)(1 + y)

Finally, summarizing the results, we formulate the initial conditions to the system of Equations (20)–(26): 2(2 − x)N N (0) = , (28) 1 1 − x 2yN N (0) = , (29) 2 (1 − x)(1 + y) xN N (0) = , (30) 3 1 − x 2(1 − y)N N (0) = , (31) 4 (1 − x)(1 + y)

N5(∞) = N, (32) xN N (∞) = , (33) 6 1 − x (1 + x − (1 − x)y)N N (∞) = . (34) 7 (1 − x)(1 + y) Condens. Matter 2021, 6, 3 7 of 13

6. Converting Problem into Dimensionless Form It is expedient to analyze the problem in dimensionless form. Let us denote:

4k κ ≡ 4 , (35) k1 p τ ≡ k1k4Nt, (36) N (t) n (τ) ≡ i . (37) i N In dimensionless kinetic-parameter κ, time-argument τ, and unknown concentration- functions ni(τ), the system of equations describing chemical kinetics takes the following form: dn1(τ) √ 4 = −2 κn (τ)n2(τ) − √ n2(τ)n3(τ), (38) dτ 1 κ √ dn (τ) κ 2 = − n (τ)n (τ), (39) dτ 2 1 2

dn3(τ) 2 = − √ n2(τ)n3(τ), (40) dτ κ

dn4(τ) 4 = − √ n2(τ)n3(τ), (41) dτ κ √ dn (τ) κ 5 = + n (τ)n (τ), (42) dτ 2 1 2

dn6(τ) 2 = + √ n2(τ)n3(τ), (43) dτ κ

dn7(τ) 4 = + √ n2(τ)n3(τ). (44) dτ κ The initial conditions for these dimensionless equations are:

2(2 − x) n ≡ n (0) = , (45) 01 1 1 − x 2y n ≡ n (0) = , (46) 02 2 (1 − x)(1 + y) x n ≡ n (0) = , (47) 03 3 1 − x 2(1 − y) n ≡ n (0) = , (48) 04 4 (1 − x)(1 + y)

n∞5 ≡ n5(∞) = 1, (49) x n ≡ n (∞) = , (50) ∞6 6 1 − x (1 + x − (1 − x)y) n ≡ n (∞) = . (51) ∞7 7 (1 − x)(1 + y) These conditions are formulated such that they guarantee the ﬁnal concentrations of reagents n∞1 ≡ n1(∞), n∞2 ≡ n2(∞), n∞3 ≡ n3(∞), n∞4 ≡ n4(∞) and the initial concentrations of products n05 ≡ n5(0), n06 ≡ n6(0), n07 ≡ n7(0) equalzero in the frames of numerical calculation errors:

n∞1 = n∞2 = n∞3 = n∞4 = n05 = n06 = n07 ≈ 0. (52) Condens. Matter 2021, 6, 3 8 of 13

Note that the subsystem of Equations (38), (39) and (40) can be resolved independently as they contain only three unknown functions n1(τ), n2(τ), and n3(τ). When these func- tions are found, the rest of the unknown functions are easily determinable from the rest of equations of full system. Excluding functions n1(τ) and n2(τ), we obtain the equation determining the function n3(τ): √ 2 1−κ ! 1+κ dn3(τ) κn3(τ) n01 n03 n3 (τ) + + κ − √ = 0. (53) dτ 1 − κ 2n03 1 − κ κ

Its solution is: 0 Z n3(τ) dn τ(n3) = − √ . (54) 02 n1−κ 01+κ n03 κn n01 03 n√ − + κ − − 1 κ 2n03 1 κ κ

In particular, for the parameter κ = 1/2, we can explicitly evaluate this integral:

n3(τ) 1 R dn0 τ(n ) = − √ = 3 02 n01 √ 03/2 2 n + √ −2 n03 n n03 2 n03 √ 2n ! (55) q 1+ 03 2 2n03 n03 2n03 n01−4n03 = − 1 + ln q . n01−4n03 n3 n01−4n03 n03 + 2n03 n3 n01−4n03

However, to obtain the explicit function n3(τ), we need to invert the latter expression for τ(n3),which is impossible. Instead, below, we solve the system of ordinary differential Equations (38)–(44) with initial Conditions (45)–(51) numerically at κ = 1/2 and; then, to check the correctness of the analytical Solution (55), we calculate that solution at discrete values of n3 obtained numerically. After that, we build an inverse plot, the discrete set of values calculated by Equation (55) vs. these discrete values of n3, together with the numerical solution for n3. If Solution (55) is correct, these two plots must coincide in the frames of numerical calculation errors.

7. Numerical Solution Code To solve Equations (38)–(44) numerically, we ﬁrst need to ﬁx the dimensionless param- eter κ contained in this set of equations. Formula (35) determines it by the ratio of reaction constants k1 and k4. On the one hand, k1 is the constant of Reaction (1), in which carbon C reacts with titanium dioxide TiO2. The chain of Reactions (1)–(3) leads to the formation of one of the ﬁnal products, namely titanium diboride TiB2. A TiB2 molecule is formed per C atom. On the other hand, 4k4 is the constant of Reaction (4), in which carbon C reacts with boron B. That reaction directly leads to the formation of other ﬁnal product, namelyboron carbide B4C. Again, a B4C molecule is formed per C atom. Thus, obtaining B4C–TiB2 compositions means that above reaction rates meet the following condition: k1 > 4k4 or 0 < κ < 1 (note that the integral in above-obtained Solution (54) is divergent at κ = 1). For test-calculations, let us take this parameter at the interval midpoint: κ = 1/2. We applied Python to solve Equations (38)–(44) numerically. More speciﬁcally, a Scipy Library was used to obtain the results and Matplotlibto draw the corresponding graphs. The methods were Odeint and Cumtrapz. First, we created the function that describes the system and returns the 1 × 3 matrix of derivatives of reduced concentrations n1, n2, and n3 of reagents. Taking κ as the ﬁxed number of 0.5, we used the relation

1 − x y = 1 + x Condens. Matter 2021, 6, 3 9 of 13

for loop to change the x parameter from 0 to 1. The y parameter that depends on x changed accordingly. For each value of parameter x, we have different initial conditions and transmit our function to the Odeint solver as an argument that gives us the solutions written as three column matrices with rows of the same number as dimensionless time-steps. Each column corresponds to the concentration of reagents for the different time values. From these three concentrations, we ﬁnd the change of the fourth reagent concentration n4 change in time with the help of Cumtrapz algorithm. We use the same scheme (Cumtrapz) to obtain the results for reduced concentrations n5, n6, and n7 of products. After that, we draw the corresponding graphs and then choose the ones that satisfy initial (ﬁnal) conditions. In addition, we compared the results to the analytical solution that we deﬁned as another function, Tau, that depends on n3 and the initial concentrations of the ﬁrst and third reagents: n01 and n03. It was impossible for us to determine analytically the solutions of n3 from the equation that contained variable Tau. Thus, to check our results, we did the inverse operation and put the values of its arguments n3, n01, and n03 into analytically obtained function Tau and compared it with the numerical solution of the same function. The results show that they matched perfectly.

8. Test Solutions Table1 summarizes the initial conditions used in numerical solutions.

Table 1. Initial and final reduced concentrations of reagents n0i and products n∞i, respectively, at different stoichiometric ratio x of synthesized (B4C)1−x(TiB2)x composite.

Condens. Matter 2021x, 6, x FOR PEER0.1 REVIEW 0.2 0.3 0.4 0.5 0.6 0.79 of 13 0.8 0.9

n01 4.22 4.50 4.86 5.33 6.00 7.00 8.67 12.00 22.00 n02 1.00Table 1. Initial 1.00 and final reduced 1.00 concentrations 1.00 of reagents 1.00 𝑛 and products 1.00 𝑛, respectively, 1.00 at 1.00 1.00 different stoichiometric ratio 𝑥 of synthesized (B4C)1–x(TiB2)x composite. n03 0.11 0.25 0.43 0.67 1.00 1.50 2.33 4.00 9.00 𝒙 0.1 0.2 0.3 0.4 0.5 0.6 0.7 0.8 0.9 n04 0.22 0.50 0.86 1.33 2.00 3.00 4.67 8.00 18.00 𝑛 n 1.00 1.004.22 4.50 1.004.86 5.33 1.00 6.00 1.007.00 8.67 1.00 12.00 1.0022.00 1.00 1.00 ∞5 𝑛 1.00 1.00 1.00 1.00 1.00 1.00 1.00 1.00 1.00 n∞6 0.11𝑛 0.250.11 0.25 0.430.43 0.67 0.67 1.00 1.001.50 2.33 1.50 4.00 2.339.00 4.00 9.00 𝑛 0.22 0.50 0.86 1.33 2.00 3.00 4.67 8.00 18.00 n∞7 0.22 0.50 0.86 1.33 2.00 3.00 4.67 8.00 18.00 𝑛 1.00 1.00 1.00 1.00 1.00 1.00 1.00 1.00 1.00 𝑛 0.11 0.25 0.43 0.67 1.00 1.50 2.33 4.00 9.00 𝑛 0.22 0.50 0.86 1.33 2.00 3.00 4.67 8.00 18.00 The corresponding curves are presented in Figure1. The corresponding curves are presented in Figure 1.

𝑥 = 0.1 𝑥 = 0.2 𝑥 =0.3

𝑥 = 0.4 𝑥 = 0.5 𝑥 =0.6

𝑥 = 0.7 𝑥 = 0.8 𝑥 =0.9 Figure 1. Calculated time-dependences of reagents and products concentrations at different stoichiometric ratio 𝑥 of synthesizedFigure (B4C) 1.1–x(TiBCalculated2)x composite. time-dependences of reagents and products concentrations at different stoichio- metric ratio x of synthesized (B C) (TiB ) composite. As expected, the 4concentrations1−x 2 ofx reagents and products are monotonously in- creasing and decreasing functions of time, respectively. The initial concentrations of all products are zero. As for the final concentrations of reagents, in most cases, they vanish as well. However, at stoichiometric ratio 𝑥 close to 1 (𝑥0.8), their saturation levels exceed 0. The explanation seems to be related with impossibility at too high 𝑥 to meet mass balance relations for all chemical elements participating in the reactions, in partic- ular carbon.

9. Possibility of Method Extending to Other Nanocomposites To not be restricted only by boron carbide/titanium diboride nanocomposites, let us discuss the generalization possibilities of the developed method of mathematical mod-

Condens. Matter 2021, 6, 3 10 of 13

As expected, the concentrations of reagents and products are monotonously increasing and decreasing functions of time, respectively. The initial concentrations of all products are zero. As for the ﬁnal concentrations of reagents, in most cases, they vanish as well. However, at stoichiometric ratio x close to 1 (x ≥ 0.8), their saturation levels exceed 0. The explanation seems to be related with impossibility at too high x to meet mass balance relations for all chemical elements participating in the reactions, in particular carbon.

9. Possibility of Method Extending to Other Nanocomposites To not be restricted only by boron carbide/titanium diboride nanocomposites, let us discuss the generalization possibilities of the developed method of mathematical modeling of the chemical reaction kinetics taking place during production of a nanopowder material. There seem to be two different directions of such analysis: separate production of boron carbide as basic component of this class of composites and simultaneous production of components of other biphasic nanocomposites. A comprehensive review on boron carbide synthesis and consolidation methods given in [14] can serve for obtaining data explainable/interpretable within the model proposed here for the chemical synthesis of boron carbide-based nanocomposites. The main methods of boron carbide production arecarbo- or magnesiothermic reductions, synthesis from elements or polymer precursors, and vapor phase reactions. However, commercially, boron carbide is produced only by the ﬁrst two: carbothermic reduction of boric acid in electric furnace or its magnesiothermy in the presence of carbon. Our modeling method is applicable for carbothermic reduction, synthesis from elements, and synthesis from polymer precursors. Thus, it is expedient to characterize them brieﬂy. The yield of carbothermic reduction is relatively low due to losses of boron due to boron oxides formation. Despite this, carbothermic reduction is usually adopted as a commercial method because of the simple equipment and cheap raw material used. However, it is not suitable for the production of boron carbide enriched in boron isotopes because such a raw material is too expensive. The overall reaction, 4 H3BO3 + 7 C → B4C + 6 CO + 6 H2O, of carbothermic reduction of boric acid (H3BO3 (and boron trioxide B2O3) proceeds in three stages: 4 H3BO3 → 2 B2O3 + 6 H2O↑,B2O3 + 3 CO↑ → 2 B + 3 CO2↑, and 4 B + C → B4C. On heating, H3BO3 converts into B2O3 (releasing water (H2O vapor), reduction of which with CO is thermodynamically feasible above 1400 ◦C. However, the temperature in the reaction area is usually maintained at higher temperatures, ~2000 ◦C, to enhance the reaction rate as the boron carbide formation is a highly endothermic process (needing 16,800 kJ/mol). According to the thermodynamic studies of gas phase carbothermic reduction of boron anhydride, B2O2 and BO are formed from B2O3 in reactions B2O3 + C → B2O2 + CO and B2O3 + C → 2 BO + CO and then reduced to free boron or target product—boron carbide. In particular, B4C nanopowders can be prepared by reduction of B2O3 vapor by carbon black at 1350 ◦C. Synthesis from elements is mostly considered as a non-commercial route of boron carbide production due to the high cost of elemental boron. It is preferred only for obtaining chemically very pure or enriched in B-isotopes boron carbides. In this technology, B and C powders are mixed to form an almost homogeneous mixture, pellets of which are then reacted at temperatures of >1500 ◦C in vacuum or inert atmosphere. There are some reported attempts of the preparation of nanostructure boron carbide in this way. Synthesis of boron carbide from polymer precursors is an alternative to the above- described high temperature techniques. Some B-containing organic compounds such as carborane(C2BnHn+2), triphenylborane, polyvinyl pentaborane, borazine, etc. on pyrolysis ◦ in the temperature range 1000–1500 C in vacuum or inert atmosphere yield B4C powder. In addition, a free-ﬂowing boron carbide powder can be obtained from boric acid and sugar mixture dissolved in ethylene glycol, dried in air at ~180 ◦C, and then heated in hydrogen at ~700 ◦C. Condens. Matter 2021, 6, 3 11 of 13

Reaction kinetics and, consequently, quality of B4C product are strongly affected by the feed charge porosity/dispersity, chemical composition, type of carbon used, heat- ing/cooling rates, and treatment temperature and duration in the reactor core. A compar- ative summary of details of various experimental data summarized in [14] can serve for reﬁnement reaction constants needed for mathematical modeling of the chemical technolo- gies for obtaining boron carbide powders. As for the biphasic nanocomposites, below, we consider the case of functional composi- tions of strongly correlated electron oxides, materials with important potential applications in spintronics and energy devices. Recently, a low-temperature (and thus also low-cost) and scalable sol-based synthesis route has been reported [15] for prototypical bimagnetic LaFeO3–CoFe2O4 (LFO–CFO) nanocomposites. In the corresponding reaction mechanism, both phases are formed simul- taneously and the CFO heat of formation assists the LFO phase crystallization. Besides, a symbiotic phenomenon is observed: LFO matrix restricts the growth of CFO particles. In this technology, at ﬁrst, two separate sols are prepared by dissolving at room temperature the precursors of LFO (La(NO3)3·6H2O and Fe(NO3)3·9H2O) and CFO (Co(NO3)2·6H2O and Fe(NO3)3·9H2O) in distilled water added with glycine acting as the chelating agent. These two solutions are mixed, and then the composite sol is heated to 80 ◦C. Next, the temperature is increased and maintained at 150 ◦C until the formation of a gel. Finally, the temperature is increased up to 250 ◦C, when a self-combustion reaction occurs and yields a powder product. Multiferroic Pb(Zr,Ti)O3–CoFe2O4 (PZT–CFO) nanocomposites have been prepared [16] in a similar synthesis technique that maximizes the surface contact area and, hence, interfacial coupling between the ferroelectric (PZT) and ferrimagnetic (CFO) phases. First, sols of PZT and CFO are prepared separately. PZT precursor solution is prepared by dissolving at room temperature lead acetate (Pb(CH3CO2)2·3H2O), zirconium propoxide (Zr(CH2CH2CH3O) and titanium isopropoxide (Ti(OCH(CH3)2) in 2-methoxyethanol and acetic acid, and then zirconium propoxide and titanium isopropoxide are added. Similarly, CFO precursor solution is prepared by dissolving at room temperature cobalt acetate tetrahydrate ((CH3COO)2Co·4H2O) and iron nitrate nonahydrate (Fe(NO3)3·9H2O) in 2-methoxyethanol and acetic acid, and then ethanolamine and ethanolamine are added. The mixed precursor solution is ﬁrst stirred at room temperature and then at 80 ◦C. Next, the temperature is increased and maintained at ~150 ◦C until the gel formation. Then, the temperature is increased to ~300 ◦C, when a self-combustion reaction occurs yielding a powder. In such biphasic composite, PZT component can be replaced [17] by strontium hex- aferrite (SrFe12O19) (SFO) component, also prepared by the sol–gel combustion. First, Fe(NO3)3·9H2O and Sr(NO3)2·6H2O precursors are dissolved in deionized water. Then, a citric acid aqueous dispersion is added at room temperature. NH3 is added drop-wise. Next, sol is heated to 80 ◦C to form a gel. After the entire solution is converted into a gel, the temperature is increased to 300 ◦C inducing self-combustion and obtaining the dry pow- ders. This sol–gel synthesis procedure can be directly adapted to simultaneously prepare the exchange-coupled hard/soft biphasic nanocomposite SrFe12O19–CoFe2O4 (SFO–CFO). Thus, sol–gel self-combustion synthesis is an efﬁcient and reproducible approach to synthesize biphasic nanocomposites. Optimizing of the synthesis conditions decreases the thermal treatment temperature, allows controlling the nanocrystallites size, and, in this way, improves the product quality. These nanocomposites reveal synthesis conditions and charge composition effect on their magnetic properties. Despite the radical differences in chemical compositions, the obtained technologies of two biphasic nanocomposite powders, such as boron carbide/titanium diboride and strongly correlated electron oxides, show similarities to each other: both materials are obtained as a result of multi-stage heat-treatments of sol charges—precursors solved in water and liquid organic compounds. Therefore, if we write down the kinetic equations for the chemical reactions occurring during the sol–gel synthesis of strongly correlated electron Condens. Matter 2021, 6, 3 12 of 13

oxides (LFO–CFO, PZT–CFO, SFO–CFO, etc.) [15–17], then the mathematical modeling of this technology can be carried out using the method developed by us for the synthesis of boron carbide/titanium diboride nanocomposite powders.

10. Concluding Remarks In summary, based on the analysis of mechanisms of chemical reactions taking place during synthesis from liquid charge of the nanopowder composites of boron carbide and titanium diboride, a system of ordinary differential equations simulating kinetics of this technology is suggested. B, C, TiO2, and CO are considered as reagents, while the expected products are B4C, TiB2, and CO2. This set of equations is resolved numerically for a typical ratio of reaction constants at different stoichiometric ratios x of components B4C and TiB2 in target composites (B4C)1−x(TiB2)x. In this way, reagent and product concentrations are found as time- functions. As expected, the concentrations of reagents and products are monotonously increasing and decreasing functions of time, respectively. The correctness of the specially elaborated computing code is proved by perfect matching of an analytical solution with the corresponding numerical one. This method of mathematical modeling will lead to the optimization of parameters of production technology of hard nanocomposites based on boron carbide. Besides, it can be extended to separate production of boron carbide as basic component of this class of composites, as well as synthesizing other biphasic nanocomposites.

Author Contributions: Conceptualization, L.C. and R.C.; methodology, L.C.; software, L.A. and L.D.; validation, L.A. and L.D.; formal analysis, L.C. and R.C.; investigation, O.T. and A.M.; resources, O.T.; data curation, A.M.; writing—original draft preparation, L.C., L.A. and L.D.; writing—review and editing, L.C.; visualization, L.A. and L.D.; supervision, L.C.; project administration, L.C. and O.T.; funding acquisition, L.C., O.T. and A.M. All authors have read and agreed to the published version of the manuscript. Funding: This research was funded by Shota Rustaveli National Science Foundation of Georgia, grant number AR–18–1045: “Obtaining of boron carbide-based nanostructured heterophase ceramic materials and products with improved performance characteristics”. Conﬂicts of Interest: The authors declare no conﬂict of interest.

References 1. Chkhartishvili, L.; Mikeladze, A.; Tsagareishvili, O.; Gachechiladze, A.; Oakley, A.; Margiev, B. Boron-Containing Nanocrystalline Ceramic and Metal-Ceramic Materials. In Handbook of Nanomaterials for Industrial Applications; Hussain, C.M., Ed.; Elsevier: Amsterdam, The Netherlands, 2018; pp. 13–35. 2. Tsagareishvili, O.; Mikeladze, A.; Chedia, R.; Chkhartishvili, L. Method of Obtaining Boron Carbide Based Hard Nanocomposite Materials. National Center for Intellectual Property of Georgia “Geo Patent”—Patent # GE P 2018 6709 B, 11 October 2018. (In Georgian). 3. Mikeladze, A.; Tsagareishvili, O.; Chkhartishvili, L.; Chedia, R.; Darchiashvili, M. Production of titanium-containing metal- ceramic composites based on boron carbide in the nanocrystalline state. Adv. Appl. Ceram. 2019, 118, 196–208. [CrossRef] 4. Mikeladze, A.; Tsagareishvili, O.; Chkhartishvili, L.; Chedia, R. Obtaining of some boron-containing and related nanocrystalline systems from solutions and suspensions. In Proceedings of the Book of International Symposium on Boron, Nevsehir, Turkey, 17–19 April 2019; pp. 181–191. 5. Barbakadze, N.; Sarajishvili, K.; Chedia, R.; Chkhartishvili, L.; Tsagareishvili, O.; Mikeladze, A.; Darchiashvili, M.; Ugrekhelidze, V. Obtaining of ultraﬁne powders of some boron carbide based nanocomposites using liquid precursors. Nanotechnol. Percept. 2019, 15, 1–14. 6. Chkhartishvili, L.; Mikeladze, A.; Chedia, R.; Tsagareishvili, O.; Barbakadze, N.; Sarajishvili, K.; Darchiashvili, M.; Ugrekhelidze, V.; Korkia, T. Synthesizing ﬁne-grained powders of complex compositions B4C–TiB2–WC–Co. Solid State Sci. 2020, 108, 1–8. [CrossRef] 7. Bogomazova, N.V. Modeling and Optimization of Chemical-Technological Processes in Industry; Belarus State Technology University: Minsk, Belarus, 2018; 83p. (In Russian) 8. Stromber, A.G.; Semchenko, D.P. Physical Chemistry; Higher Schoo: Moscow, Russia, 1988; 496p. (In Russian) 9. Tsagareishvili, G.V.; Antadze, M.E.; Tavadze, F.N. Obtaining and Structure of Boron; Metsniereba: Tbilisi, Georgia, 1991; 144p. (In Russian) Condens. Matter 2021, 6, 3 13 of 13

10. Chkhartishvili, L. Relative stability of planar clusters B11, B12, and B13 in neutral- and charged-states. Charact. Appl. Nanomater. 2018, 2, 1–7. [CrossRef] 11. Lifshitz, C. Carbon clusters. Int. J. Mass Spectrom. 2000, 200, 423–442. [CrossRef] 12. Schröder, D.; Schwarz, H.; Dua, S.; Blanksby, S.J.; Bowie, J.H. Mass spectrometric studies of the oxocarbons CnOn (n = 3–6). Int. J. Mass Spectrom. 1999, 188, 17–25. [CrossRef] 13. Ramana, M.V.; Phillips, D.H. A computational study of the TiO2 molecule. J. Chem. Phys. 1988, 88, 2637–2640. [CrossRef] 14. Suri, A.K.; Subramanian, C.; Sonber, J.K.; Murthy, T.S.R.C. Synthesis and consolidation of boron carbide: A review. Int. Mater. Rev. 2010, 55, 4–40. [CrossRef] 15. Sayed, F.; Kotnana, G.; Muscas, G.; Locardi, F.; Comite, A.; Varvaro, G.; Peddis, D.; Barucca, G.; Mathieu, R.; Sarkar, T. Symbiotic, low-temperature, and scalable synthesis of bi-magnetic complex oxide nanocomposites. Nanoscale Adv. 2020, 2, 851–859. [CrossRef] 16. Kotnana, G.; Sayed, F.; Joshi, D.; Barucca, G.; Peddis, D.; Mathieu, R.; Sarkar, T. Novel mixed precursor approach to prepare multiferroic nanocomposites with enhanced interfacial coupling. J. Magn. Magn. Mater. 2020, 511, 166792. [CrossRef] 17. Maltoni, P.; Sarkar, T.; Varvaro, G.; Barucca, G.; Ivanov, S.; Peddis, D.; Mathieu, R. Towards bi-magnetic nanocomposites as permanent magnets through the optimization of the synthesis and magnetic properties of SrFe12O19 nanocrystallites. J. Phys. D Appl. Phys. 2020.[CrossRef]